Scalable synthesis of a biocompatible, transparent and superparamagnetic photoresist for microdevice fabrication
This content has been downloaded from IOPscience. Please scroll down to see the full text. 2013 J. Micromech. Microeng. 23 107002 (http://iopscience.iop.org/0960-1317/23/10/107002) View the table of contents for this issue, or go to the journal homepage for more Download details: IP Address: 220.127.116.11 This content was downloaded on 09/06/2017 at 20:12 Please note that terms and conditions apply.
You may also be interested in: Characterization of freestanding photoresist films for biological and MEMS applications D M Ornoff, Y Wang and N L Allbritton The preparation of magnetically guided lipid based nanoemulsions using self-emulsifyingtechnology Aristides Bakandritsos, Radek Zboril, Nikolaos Bouropoulos et al. Interactions between sub-10-nm iron and cerium oxide nanoparticles and 3T3 fibroblasts:the role of the coating and aggregation state M Safi, H Sarrouj, O Sandre et al. Patterned cell arrays and patterned co-cultures on polydopamine-modified poly(vinyl alcohol) hydrogels Kai M Beckwith and Pawel Sikorski Functionalized [email protected]
superparamagnetic nanoparticles: in vitro bioactivity J Salado, M Insausti, L Lezama et al. Poly(ethylene oxide)-block-poly(glutamic acid) coated maghemite nanoparticles: in vitrocharacterization and in vivo behaviour L Kaufner, R Cartier, R Wüstneck et al. ‘Green’-synthesized near-infrared PbS quantum dots with silica–PEG dual-layer coating: ultrastable and biocompatible optical probes for in vivo animal imaging D Wang, J Qian, F Cai et al. Magnetite/CdTe magnetic–fluorescent composite nanosystem for magnetic separation andbio-imaging Anup Kale, Sonia Kale, Prasad Yadav et al.
JOURNAL OF MICROMECHANICS AND MICROENGINEERING
J. Micromech. Microeng. 23 (2013) 107002 (7pp)
Scalable synthesis of a biocompatible, transparent and superparamagnetic photoresist for microdevice fabrication P K Shah 1 , M R Hughes 2 , Y Wang 2 , C E Sims 2 and N L Allbritton 1,2 1
Department of Biomedical Engineering, University of North Carolina, Chapel Hill, NC 27599, USA and North Carolina State University, Raleigh, NC 27695, USA 2 Department of Chemistry, University of North Carolina, Chapel Hill, NC 27599, USA E-mail: [email protected]
Received 12 June 2013, in final form 18 August 2013 Published 11 September 2013 Online at stacks.iop.org/JMM/23/107002 Abstract The functionalization of photoresists with colloids has enabled the development of novel active and passive components for microfabricated devices. Incorporation of colloidal particles often results in undesirable reductions in photolithographic fidelity and device transparency. We present a novel photoresist composite incorporating poly(methyl methacrylate-co-methacrylic acid), the epoxy resin 1002F and colloidal maghemite nanoparticles to produce a stable, transparent and biocompatible photoresist. The composite photoresist was prepared in a scalable fashion in batches up to 1 kg with the particles remaining dispersed during room-temperature storage for at least six months. Following photolithography to form films, the nanoparticle size remained well below that of visible-light wavelengths as demonstrated by electron microscopy. Structures fabricated from the photoresist by conventional photolithography displayed aspect ratios greater than ten. When grown on the photoresist, the metabolic rate of HeLa cells was unchanged relative to cells grown on glass. Primary murine mesenchymal stem cells also displayed a normal morphology on the resist surface. The ability to manipulate microstructures formed from the composite was demonstrated by magnetically collecting clonal colonies of HeLa cells from a micropallet array. The transparency, biocompatibility, scalable synthesis and superparamagnetic properties of the novel composite address key limitations of existing magnetic composites. (Some figures may appear in colour only in the online journal)
of on-chip optical waveguides . These composites have typically relied upon the addition of insoluble components, often nanoparticles, into the photoresist. A common feature among nanocomposites incorporating metallic colloids is reduced accuracy in reproducing mask features, diminished fabrication quality and poor optical clarity. This undesirable optical property is generally due to an uneven distribution of the colloid in the photoresist as a result of aggregation. For biological applications where optical clarity is critical for analysis and imaging, transparent nanocomposite photoresists would prove valuable. Gach et al  demonstrated a method
The generation of nanocomposite photoresists with modified properties has dramatically expanded the toolbox available for the integration of active and passive components into microdevices. Nanocomposites have been developed to confer properties of ferro- and superparamagnetism for mechanically actuatable devices [1–5], conductivity for the integration of electrodes [6–9], high dielectric constants for integrated capacitors , low internal stress for improving mechanical properties  and a low index of refraction for the generation 0960-1317/13/107002+07$33.00
© 2013 IOP Publishing Ltd
Printed in the UK & the USA
J. Micromech. Microeng. 23 (2013) 107002
for dispersing iron oxide nanoparticles in photoresist that yielded high-fidelity, optically clear structures. This method, however, required high-intensity ultrasonication to prevent nanoparticle aggregation and was not amenable to production in large batches. In addition, the resulting photoresist was limited to aspect ratios of 4:1, offering no improvement in mechanical properties over the native 1002F photoresist it was based upon . To address these issues, we present a novel photoresist composite incorporating the epoxide-based photoresist 1002F and poly(methyl methacrylate-co-methacrylic acid) (PMMA/MMA). To test the photolithographic performance of the PMMA/1002F-based photoresist, arrays of microposts of varying diameters were fabricated and imaged by scanning electron microscopy (SEM). The dispersion of the maghemite nanoparticles in the PMMA/1002F composite was evaluated by imaging 100 nm thick sections of the cross-linked composite by transmission electron microscopy (TEM). The spectral transmittance of the 0.25% (w/w) maghemite PMMA/1002F composite was measured by UV–vis spectroscopy and the reaction of PMMA/MMA with the 1002F epoxy was confirmed by differential scanning calorimetry (DSC). The effect of the maghemite PMMA/1002F composite surface on cellular metabolism was tested by tracking the metabolic activity of HeLa cells over 72 h. Additionally, the compatibility of the composite surface with primary cell culture was evaluated by culturing murine mesenchymal stem cells (MSC) for 72 h and observing cell morphology. The functionality of the magnetic composite was assessed by isolating single adherent cells cultured on an array of individually removable magnetic cell carriers [14, 15].
and weighing the dry solids. PMMA/MMA (100 g of methyl methacrylate:methacrylic acid at a molar ratio of 1:0.016, PMMA/MMA molecular weight = 34 000, Sigma Aldrich, St Louis, MO) was added to the nanoparticle solution and allowed to dissolve overnight while stirring. γ -butyrolactone (233.3 g) was added drop-by-drop using a separatory funnel and stirred further for an additional 24 h. The toluene in the solution was then removed by rotoevaporation at 60 ◦ C leaving a deep red, highly viscous polymer suspension. The superparamagnetic PMMA/MMA solution was then added directly to 1002F-50 photoresist (1:2.6 by mass, PMMA/MMA:1002F-50) which had been prepared as previously described . The mixture was then placed on a bottle roller for four days. The resulting PMMA/1002F photoresist was deep red in color. 2.3. Characterization of PMMA/1002F photoresist and magnetic composite Melting point and glass transition temperatures were determined by DSC with a Q200 calorimeter (TA Instruments, New Castle, DE). 1002F and PMMA/MMA samples were analyzed as pure powders packed into the DSC sample pans. The PMMA/1002F was analyzed after 100 μL of the polymer suspension was baked into the sample pan at 120 ◦ C for 72 h under vacuum to completely remove the solvent. For optical characterization, 50 μm thick films of 1002F photoresist, PMMA/1002F, and PMMA/1002F with 0.25% (w/w) maghemite nanoparticles were prepared by spin coating onto plasma-cleaned glass coverslips. These films were treated as described below for micropallet fabrication before use except that no mask was used in producing UV-cross-linked films. Transmission spectra for triplicate preparations of each film were measured with a bare coverslip as a blank using a SpectraMax M5 spectrophotometer (Molecular Devices Corporation, Sunnyvale, CA). Working curves were generated by producing films of different thickness by varying the speed of the spin-coat step. The exposure needed to fully cross-link the films and form microstructures was then optimized and the final thickness of the film measured using a P-6 stylus profilometer (KLA Tencor, Milpitas, CA). The maximum aspect ratio of the PMMA/1002F with 0.25% maghemite nanoparticles composite was determined by fabricating a post-array using the protocol described below for fabrication of micropallet arrays. The fabricated structures were then imaged by SEM using a Quanta 200 environmental-SEM (FEI, Hillsboro, OR). The dispersion of maghemite nanoparticles into the PMMA/1002F photoresist was characterized by imaging transverse slices of a 50 μm thick film of the magnetic PMMA/1002F composite photoresist by TEM (JEOL 100CX II). The film was set in Polybed 812 resin and cured at 65 ◦ C overnight. 100 nm thick sections of the film were cut with an ultramicrotome prior to imaging.
2. Methods 2.1. Synthesis of maghemite nanoparticles A solution of 10 nm maghemite nanoparticles in toluene was prepared using the method described by Gach et al . Iron salts (23.82 g FeCl2 and 38.94 g FeCl3 in 3 L of deionized (DI) water) were precipitated by the addition of a strong base (240 mL of 14.5 M NH4OH), and washed three times with DI water by magnetic decantation. After resuspension in 480 mL of 1.5 M HNO3, 104 g of Fe(NO3)2 was added to the solution which was then heated to boiling for 1 h. After cooling to 25 ◦ C the precipitate was washed by magnetic decantation once with 480 mL of 1.5 M HNO3, once with 2500 mL of 0.1 M NH4OH and resuspended in 1500 mL of DI water. 90 g of oleic acid was added to the suspension and mixed for 15 min. The excess oleic acid and water were removed from the precipitate by three successive extractions with 200 mL of 100% ethanol. The precipitate was then dissolved in 800 mL of toluene and stored in amber glass bottles until use. 2.2. Composite preparation
2.4. Cell culture and proliferation assay
Maghemite nanoparticles (3 g) were diluted with toluene (800 mL total volume). The weight percentage of maghemite nanoparticles in toluene was determined by evaporating solvent from a sample by heating at 120 ◦ C for 30 min
Uniform films of PMMA/MMA, 1002F-50 and PMMA/1002F with 0.25% (w/w) maghemite nanoparticles as well as bare glass slides were treated with an air 2
J. Micromech. Microeng. 23 (2013) 107002
Biosciences, San Jose, CA) which had been treated with air plasma for 10 min and sterilized using the protocol described above. The magnetic collection experiment was carried out as described by Gach et al . The clonal colonies were released by focusing a 5 ns pulse from an Nd:YAG laser at the photoresist–glass interface through a 20 × , 0.7 N.A. objective and collected against gravity by a ring-shaped rare earth magnet (K&J Magnetics) placed on the collection plate. The cassette was designed to reduce the gap between the array and the collection plate to 3 mm. After collection, the Petri dish was removed from the cassette with the magnet, inverted and filled with an expansion media consisting of 50% FBS, 25% HeLa-GFP conditioned DMEM and 25% fresh DMEM. The conditioned media was generated by incubating 20 mL of fresh DMEM on a culture of HeLa cells on a 75 mm2 tissue culture flask at 50% confluency for 24 h. The conditioned media was then aspirated and filtered through a 0.22 μm nylon filter and stored at 4 ◦ C for less than 72 h before use. The released clonal colonies were imaged again after three days to confirm their viability and to observe the expansion of the colony onto the Petri dish surface.
plasma (Harrick Plasma, Ithaca, NY) for 5 min after being affixed to 4-well arrays fabricated from polylactic acid with a benchtop 3D-printer (BFB-3000, Bits from Bytes Inc., Clevedon, UK). Polydimethylsiloxane (PDMS) was used to glue the wells to the surfaces. HeLa cells were plated in three of four wells of each array at a density of 2000 cells per well in 100 μL of culture media and cultured for 24, 48 or 72 h. Medium in each well was replaced every 24 h. A standard cell proliferation assay (MTT) was performed at multiple time points in accordance with the manufacturer’s instructions (Life Technologies, Grand Island, NY). Briefly, 10 μL of 5 mg mL−1 3-(4,5-dimethylthiazol-2-yl)-2,5diphenyltetrazolium bromide (MTT) was added to each of three sample wells and one control well containing no cells and incubated at 37 ◦ C for 4 h. MTT is metabolized by cells into an insoluble purple formazan which is then solubilized by the addition of 100 μL of 100 mg mL−1 sodium dodecyl sulfate in 0.01 M HCl followed by incubation at 37 ◦ C for 4 h. 100 μL of fluid from each well was sampled and absorbance measurements were taken at 570 nm using a spectrophotometer. To test the compatibility of the composite with primary cell growth, MSC were derived from the long bone of a mouse  and plated on conventional tissue-culture dishes or films of the magnetic PMMA/1002F composite in Dulbecco’s modified Eagle medium (DMEM) with 10% fetal bovine serum and cultured for 72 h.
3. Results 3.1. Characterization of PMMA/1002F photoresists Previous protocols to stably disperse maghemite nanoparticles into pure 1002F photoresist proved difficult to scale. Polymer additives were explored for their potential to stabilize the maghemite nanoparticles while forming a single phase with the photoresist. PMMA/MMA was selected as an additive to the 1002F photoresist system for its optical clarity, high glass transition temperature and the presence of acidic groups which could react with epoxides in the 1002F as well as stabilize the nanoparticles. The glass transition of PMMA/MMA occurred at 110 ◦ C (figure 1(A)). Un-cross-linked 1002F was observed to melt at 56.8 ◦ C. When a mixture of PMMA/MMA and 1002F was heated from 40 to 140 ◦ C, the material did not melt and a single glass transition was observed at 110 ◦ C, supporting the conclusion that covalent bonds were formed between the 1002F and PMMA/MMA to form a single phase. In order to maintain optical clarity for imaging and photolithographic fidelity, maghemite nanoparticles